#------------------------------------------------------------------------------
#$Date: 2016-03-23 00:19:13 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179104 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/66/4306607.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4306607
loop_
_publ_author_name
'Céline Pichon'
'Pierre Mialane'
'Anne Dolbecq'
'Jérôme Marrot'
'Eric Rivière'
'Bassem S. Bassil'
'Ulrich Kortz'
'Bineta Keita'
'Louis Nadjo'
'Francis Sécheresse'
_publ_contact_author
; 
      Dr P. Mialane
      Institut Lavoisier de Versailles, UMR 8180
      Université de Versailles Saint-Quentin-en-Yvelines
      45 Avenue des Etats Unis
      78035 Versailles cedex
      France
;
_publ_contact_author_email       mialane@chimie.uvsq.fr
_publ_contact_author_fax         '(33) 1 39 25 43 81'
_publ_contact_author_phone       '(33) 1 39 25 43 83'
_publ_section_title
;
Octa- and Nonanuclear Nickel(II) Polyoxometalate Clusters: Synthesis and
Electrochemical and Magnetic Characterizations
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              11120
_journal_page_last               11128
_journal_paper_doi               10.1021/ic801431f
_journal_volume                  47
_journal_year                    2008
_chemical_formula_sum            'C12 H18 Cl4 Na20 Ni8 O115.5 Si2 W18'
_chemical_formula_weight         6447.02
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           163
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-P 3 2c'
_symmetry_space_group_name_H-M   'P -3 1 c'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   11.92720(10)
_cell_length_b                   11.92720(10)
_cell_length_c                   48.4712(11)
_cell_measurement_reflns_used    7147
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      30.04
_cell_measurement_theta_min      2.34
_cell_volume                     5971.61(15)
_computing_cell_refinement       'Bruker APEX2'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 512x512
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0488
_diffrn_reflns_av_sigmaI/netI    0.0233
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       68
_diffrn_reflns_limit_l_min       -68
_diffrn_reflns_number            70171
_diffrn_reflns_theta_full        30.06
_diffrn_reflns_theta_max         30.06
_diffrn_reflns_theta_min         0.84
_exptl_absorpt_coefficient_mu    18.786
_exptl_absorpt_correction_T_max  0.7051
_exptl_absorpt_correction_T_min  0.0784
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, V2.10)'
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    3.585
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       parallelepiped
_exptl_crystal_F_000             5772
_exptl_crystal_size_max          0.14
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.02
_refine_diff_density_max         4.023
_refine_diff_density_min         -8.510
_refine_diff_density_rms         1.016
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.095
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     272
_refine_ls_number_reflns         5845
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.095
_refine_ls_R_factor_all          0.0858
_refine_ls_R_factor_gt           0.0773
_refine_ls_shift/su_max          0.004
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0722P)²+1336.5593P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2133
_refine_ls_wR_factor_ref         0.2342
_reflns_number_gt                5340
_reflns_number_total             5845
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic801431f_si_003_1.cif
_cod_data_source_block           1
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Trigonal' changed to 'trigonal' according
to '/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_database_code               4306607
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-y, -x, -z+1/2'
'-x+y, y, -z+1/2'
'x, x-y, -z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'y, x, z-1/2'
'x-y, -y, z-1/2'
'-x, -x+y, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.66123(3) 0.16650(3) 0.533252(6) 0.01402(7) Uani 1 1 d . . .
W2 W 0.84000(3) 0.16291(3) 0.596427(6) 0.01551(7) Uani 1 1 d . . .
W3 W 1.00788(3) 0.48645(3) 0.597307(6) 0.01579(7) Uani 1 1 d . . .
Ni1 Ni 0.84076(9) 0.32537(10) 0.64902(2) 0.0170(2) Uani 1 1 d . . .
Ni2 Ni 0.6667 0.3333 0.68984(4) 0.0186(4) Uani 1 3 d S . .
Si1 Si 0.6667 0.3333 0.59407(6) 0.0058(6) Uani 1 3 d S . .
O1 O 0.6617(6) 0.0620(6) 0.50871(12) 0.0212(14) Uani 1 1 d . . .
O2 O 0.5329(5) 0.0543(5) 0.55719(11) 0.0179(15) Uani 1 1 d . . .
O3 O 0.7880(5) 0.1789(5) 0.55764(11) 0.0180(15) Uani 1 1 d . . .
O4 O 0.5371(5) 0.2062(5) 0.51675(12) 0.0176(14) Uani 1 1 d . . .
O5 O 0.6667 0.3333 0.5597(2) 0.0212(14) Uani 1 3 d S . .
O6 O 0.8895(6) 0.0532(6) 0.58792(14) 0.0274(16) Uani 1 1 d . . .
O7 O 0.8718(5) 0.1841(6) 0.63282(13) 0.0211(16) Uani 1 1 d . . .
O8 O 0.6580(6) 0.0512(5) 0.60102(11) 0.0195(15) Uani 1 1 d . . .
O9 O 0.9981(5) 0.3231(5) 0.58732(12) 0.0190(15) Uani 1 1 d . . .
O10 O 0.7958(5) 0.3314(5) 0.60497(12) 0.0171(14) Uani 1 1 d . . .
O11 O 1.1691(6) 0.5887(7) 0.58953(14) 0.0285(19) Uani 1 1 d . . .
O12 O 1.0159(5) 0.4633(5) 0.63359(12) 0.0194(15) Uani 1 1 d . . .
O13 O 0.8019(5) 0.4608(6) 0.66267(12) 0.0208(14) Uani 1 1 d . . .
O14 O 0.9362(6) 0.3223(6) 0.68458(13) 0.0247(16) Uani 1 1 d . . .
O15 O 0.6721(7) 0.4714(6) 0.71561(13) 0.0261(17) Uani 1 1 d . . .
C1 C 0.6718(10) 0.5748(10) 0.7093(2) 0.037(2) Uani 1 1 d . . .
C2 C 0.6579(10) 0.6536(10) 0.73215(19) 0.037(2) Uani 1 1 d . . .
H2A H 0.6188 0.5995 0.7480 0.055 Uiso 1 1 calc R . .
H2B H 0.6043 0.6875 0.7259 0.055 Uiso 1 1 calc R . .
H2C H 0.7418 0.7239 0.7371 0.055 Uiso 1 1 calc R . .
Na1 Na 1.3333 0.6667 0.56131(10) 0.0051(9) Uani 1 3 d S . .
Na2 Na 0.6667 0.3333 0.7500 0.034(3) Uani 1 6 d S . .
Na3 Na 0.6813(4) 0.0052(4) 0.46302(7) 0.0426(10) Uani 1 1 d . . .
Na4 Na 0.9943(5) 0.1703(5) 0.66696(11) 0.0400(14) Uani 0.83 1 d P . .
Na5 Na 1.1623(6) 0.4939(7) 0.66961(12) 0.053(2) Uani 0.83 1 d P . .
Na6 Na 1.0000 0.0000 0.5568(4) 0.061(6) Uani 0.50 3 d SP . .
Cl1 Cl 1.0000 0.0000 0.7500 0.070(3) Uani 1 6 d S . .
Cl2 Cl 1.1237(7) 0.6609(6) 0.69714(15) 0.054(2) Uani 0.50 1 d P . .
O1W O 0.4769(10) 0.2090(7) 0.46232(14) 0.053(3) Uani 1 1 d . . .
O2W O 1.0000 0.0000 0.6387(3) 0.032(3) Uani 1 3 d S . .
O3W O 1.1699(7) 0.3302(11) 0.63812(19) 0.054(2) Uani 1 1 d . . .
O4W O 1.3333 0.6667 0.6418(2) 0.036(3) Uani 1 3 d S . .
O5W O 0.8213(8) -0.0499(13) 0.5331(2) 0.054(2) Uani 0.83 1 d P . .
O6W O 1.1640(11) 0.1730(11) 0.6973(2) 0.076(3) Uani 1 1 d . . .
O7W O 1.0000 0.0000 0.5000 0.017(6) Uani 0.50 6 d SP . .
O8W O 0.3333 0.6667 0.7500 0.14(4) Uani 0.50 6 d SP . .
O9W O 0.262(5) 0.639(6) 0.7341(18) 0.14(4) Uani 0.25 1 d P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 W1 O2 102.1(3) . . ?
O1 W1 O3 101.5(3) . . ?
O2 W1 O3 90.2(2) . . ?
O1 W1 O4 99.8(3) . . ?
O2 W1 O4 88.8(3) . . ?
O3 W1 O4 158.4(3) . . ?
O1 W1 O4 98.5(2) . 2_655 ?
O2 W1 O4 159.2(3) . 2_655 ?
O3 W1 O4 87.9(2) . 2_655 ?
O4 W1 O4 85.4(3) . 2_655 ?
O1 W1 O5 169.5(3) . . ?
O2 W1 O5 86.2(3) . . ?
O3 W1 O5 84.8(3) . . ?
O4 W1 O5 73.6(2) . . ?
O4 W1 O5 73.1(2) 2_655 . ?
O1 W1 Na3 92.1(2) . 7_656 ?
O2 W1 Na3 41.7(2) . 7_656 ?
O3 W1 Na3 131.91(17) . 7_656 ?
O4 W1 Na3 50.32(17) . 7_656 ?
O4 W1 Na3 135.67(16) 2_655 7_656 ?
O5 W1 Na3 89.85(8) . 7_656 ?
O1 W1 Na3 89.8(2) . 8_666 ?
O2 W1 Na3 131.8(2) . 8_666 ?
O3 W1 Na3 41.59(17) . 8_666 ?
O4 W1 Na3 135.33(16) . 8_666 ?
O4 W1 Na3 49.95(16) 2_655 8_666 ?
O5 W1 Na3 89.38(8) . 8_666 ?
Na3 W1 Na3 173.50(11) 7_656 8_666 ?
O6 W2 O7 102.2(3) . . ?
O6 W2 O8 101.5(3) . . ?
O7 W2 O8 94.0(2) . . ?
O6 W2 O9 99.1(3) . . ?
O7 W2 O9 93.0(2) . . ?
O8 W2 O9 156.3(3) . . ?
O6 W2 O3 95.0(3) . . ?
O7 W2 O3 162.8(3) . . ?
O8 W2 O3 83.0(2) . . ?
O9 W2 O3 83.6(2) . . ?
O6 W2 O10 172.8(2) . . ?
O7 W2 O10 80.2(3) . . ?
O8 W2 O10 85.0(2) . . ?
O9 W2 O10 73.9(2) . . ?
O3 W2 O10 82.7(2) . . ?
O6 W2 Na3 84.7(2) . 8_666 ?
O7 W2 Na3 135.65(18) . 8_666 ?
O8 W2 Na3 127.93(18) . 8_666 ?
O9 W2 Na3 42.91(19) . 8_666 ?
O3 W2 Na3 44.93(16) . 8_666 ?
O10 W2 Na3 88.93(15) . 8_666 ?
O11 W3 O12 101.4(3) . . ?
O11 W3 O8 100.9(4) . 2_655 ?
O12 W3 O8 95.3(3) . 2_655 ?
O11 W3 O9 98.1(3) . . ?
O12 W3 O9 94.1(3) . . ?
O8 W3 O9 156.7(3) 2_655 . ?
O11 W3 O2 94.2(3) . 2_655 ?
O12 W3 O2 164.4(2) . 2_655 ?
O8 W3 O2 82.1(2) 2_655 2_655 ?
O9 W3 O2 83.1(3) . 2_655 ?
O11 W3 O10 173.1(3) . . ?
O12 W3 O10 80.7(2) . . ?
O8 W3 O10 85.3(3) 2_655 . ?
O9 W3 O10 75.2(2) . . ?
O2 W3 O10 83.7(2) 2_655 . ?
O11 W3 Na3 84.7(3) . 8_666 ?
O12 W3 Na3 136.2(2) . 8_666 ?
O8 W3 Na3 126.45(17) 2_655 8_666 ?
O9 W3 Na3 42.37(18) . 8_666 ?
O2 W3 Na3 44.36(18) 2_655 8_666 ?
O10 W3 Na3 89.29(17) . 8_666 ?
O13 Ni1 O13 84.5(3) . 3_665 ?
O13 Ni1 O12 91.5(3) . . ?
O13 Ni1 O12 174.4(3) 3_665 . ?
O13 Ni1 O7 176.0(3) . . ?
O13 Ni1 O7 94.3(2) 3_665 . ?
O12 Ni1 O7 89.4(2) . . ?
O13 Ni1 O14 95.2(3) . . ?
O13 Ni1 O14 96.1(2) 3_665 . ?
O12 Ni1 O14 88.2(2) . . ?
O7 Ni1 O14 88.7(3) . . ?
O13 Ni1 O10 97.8(3) . . ?
O13 Ni1 O10 98.8(2) 3_665 . ?
O12 Ni1 O10 77.7(2) . . ?
O7 Ni1 O10 78.7(3) . . ?
O14 Ni1 O10 161.1(3) . . ?
O13 Ni1 Ni2 44.84(15) . . ?
O13 Ni1 Ni2 44.87(15) 3_665 . ?
O12 Ni1 Ni2 132.95(19) . . ?
O7 Ni1 Ni2 135.45(16) . . ?
O14 Ni1 Ni2 80.9(2) . . ?
O10 Ni1 Ni2 117.89(18) . . ?
O13 Ni1 Na4 141.4(2) . . ?
O13 Ni1 Na4 100.31(18) 3_665 . ?
O12 Ni1 Na4 85.3(2) . . ?
O7 Ni1 Na4 42.6(2) . . ?
O14 Ni1 Na4 46.3(2) . . ?
O10 Ni1 Na4 118.9(2) . . ?
Ni2 Ni1 Na4 116.40(10) . . ?
O13 Ni1 Na5 94.1(2) . . ?
O13 Ni1 Na5 142.6(2) 3_665 . ?
O12 Ni1 Na5 41.5(2) . . ?
O7 Ni1 Na5 89.1(2) . . ?
O14 Ni1 Na5 46.71(19) . . ?
O10 Ni1 Na5 118.34(17) . . ?
Ni2 Ni1 Na5 112.74(12) . . ?
Na4 Ni1 Na5 59.14(17) . . ?
O15 Ni2 O15 86.5(3) 3_665 2_655 ?
O15 Ni2 O15 86.5(3) 3_665 . ?
O15 Ni2 O15 86.5(3) 2_655 . ?
O15 Ni2 O13 94.7(3) 3_665 . ?
O15 Ni2 O13 177.6(3) 2_655 . ?
O15 Ni2 O13 95.7(3) . . ?
O15 Ni2 O13 95.7(2) 3_665 3_665 ?
O15 Ni2 O13 94.7(3) 2_655 3_665 ?
O15 Ni2 O13 177.6(3) . 3_665 ?
O13 Ni2 O13 83.1(2) . 3_665 ?
O15 Ni2 O13 177.6(3) 3_665 2_655 ?
O15 Ni2 O13 95.7(3) 2_655 2_655 ?
O15 Ni2 O13 94.7(3) . 2_655 ?
O13 Ni2 O13 83.1(2) . 2_655 ?
O13 Ni2 O13 83.1(2) 3_665 2_655 ?
O15 Ni2 Ni1 80.7(2) 3_665 . ?
O15 Ni2 Ni1 134.8(2) 2_655 . ?
O15 Ni2 Ni1 135.09(18) . . ?
O13 Ni2 Ni1 43.6(2) . . ?
O13 Ni2 Ni1 44.6(2) 3_665 . ?
O13 Ni2 Ni1 97.04(17) 2_655 . ?
O15 Ni2 Ni1 134.8(2) 3_665 2_655 ?
O15 Ni2 Ni1 135.09(17) 2_655 2_655 ?
O15 Ni2 Ni1 80.7(2) . 2_655 ?
O13 Ni2 Ni1 44.6(2) . 2_655 ?
O13 Ni2 Ni1 97.04(17) 3_665 2_655 ?
O13 Ni2 Ni1 43.6(2) 2_655 2_655 ?
Ni1 Ni2 Ni1 78.68(5) . 2_655 ?
O15 Ni2 Ni1 135.09(17) 3_665 3_665 ?
O15 Ni2 Ni1 80.7(2) 2_655 3_665 ?
O15 Ni2 Ni1 134.8(2) . 3_665 ?
O13 Ni2 Ni1 97.04(17) . 3_665 ?
O13 Ni2 Ni1 43.6(2) 3_665 3_665 ?
O13 Ni2 Ni1 44.6(2) 2_655 3_665 ?
Ni1 Ni2 Ni1 78.68(5) . 3_665 ?
Ni1 Ni2 Ni1 78.68(5) 2_655 3_665 ?
O15 Ni2 Na2 52.3(2) 3_665 . ?
O15 Ni2 Na2 52.3(2) 2_655 . ?
O15 Ni2 Na2 52.3(2) . . ?
O13 Ni2 Na2 130.01(16) . . ?
O13 Ni2 Na2 130.01(16) 3_665 . ?
O13 Ni2 Na2 130.01(16) 2_655 . ?
Ni1 Ni2 Na2 132.95(3) . . ?
Ni1 Ni2 Na2 132.95(3) 2_655 . ?
Ni1 Ni2 Na2 132.95(3) 3_665 . ?
O10 Si1 O10 110.1(2) 2_655 3_665 ?
O10 Si1 O10 110.1(2) 2_655 . ?
O10 Si1 O10 110.1(2) 3_665 . ?
O10 Si1 O5 108.8(2) 2_655 . ?
O10 Si1 O5 108.8(2) 3_665 . ?
O10 Si1 O5 108.8(2) . . ?
W1 O1 Na3 153.0(4) . . ?
W1 O2 W3 147.8(3) . 3_665 ?
W1 O2 Na3 108.6(3) . 7_656 ?
W3 O2 Na3 100.1(2) 3_665 7_656 ?
W1 O3 W2 149.1(3) . . ?
W1 O3 Na3 108.7(3) . 8_666 ?
W2 O3 Na3 100.2(2) . 8_666 ?
W1 O4 W1 120.4(3) . 3_665 ?
W1 O4 Na3 96.8(2) . 7_656 ?
W1 O4 Na3 96.7(2) 3_665 7_656 ?
Si1 O5 W1 123.2(2) . . ?
Si1 O5 W1 123.2(2) . 2_655 ?
W1 O5 W1 92.9(3) . 2_655 ?
Si1 O5 W1 123.2(2) . 3_665 ?
W1 O5 W1 92.9(3) . 3_665 ?
W1 O5 W1 92.9(3) 2_655 3_665 ?
W2 O6 Na6 145.7(4) . . ?
W2 O7 Ni1 112.3(4) . . ?
W2 O7 Na4 143.6(4) . . ?
Ni1 O7 Na4 99.6(3) . . ?
W3 O8 W2 157.8(4) 3_665 . ?
W2 O9 W3 117.9(3) . . ?
W2 O9 Na3 104.2(3) . 8_666 ?
W3 O9 Na3 105.0(3) . 8_666 ?
Si1 O10 Ni1 123.8(3) . . ?
Si1 O10 W3 126.9(3) . . ?
Ni1 O10 W3 89.70(18) . . ?
Si1 O10 W2 124.6(3) . . ?
Ni1 O10 W2 88.9(2) . . ?
W3 O10 W2 91.9(2) . . ?
W3 O11 Na1 152.1(4) . . ?
W3 O12 Ni1 111.8(3) . . ?
W3 O12 Na5 142.5(3) . . ?
Ni1 O12 Na5 103.4(3) . . ?
Ni1 O13 Ni1 131.3(3) . 2_655 ?
Ni1 O13 Ni2 91.6(2) . . ?
Ni1 O13 Ni2 90.6(3) 2_655 . ?
C1 O14 Ni1 126.2(7) 3_665 . ?
C1 O14 Na4 126.3(6) 3_665 . ?
Ni1 O14 Na4 94.9(3) . . ?
C1 O14 Na5 117.3(7) 3_665 . ?
Ni1 O14 Na5 96.8(3) . . ?
Na4 O14 Na5 85.2(3) . . ?
C1 O15 Ni2 128.3(6) . . ?
C1 O15 Na2 148.0(6) . . ?
Ni2 O15 Na2 83.6(3) . . ?
O15 C1 O14 123.8(10) . 2_655 ?
O15 C1 C2 118.6(9) . . ?
O14 C1 C2 117.5(11) 2_655 . ?
C1 C2 H2A 109.5 . . ?
C1 C2 H2B 109.5 . . ?
H2A C2 H2B 109.5 . . ?
C1 C2 H2C 109.5 . . ?
H2A C2 H2C 109.5 . . ?
H2B C2 H2C 109.5 . . ?
O11 Na1 O11 84.8(3) 3_775 2_755 ?
O11 Na1 O11 84.8(3) 3_775 . ?
O11 Na1 O11 84.8(3) 2_755 . ?
O11 Na1 O1W 82.1(3) 3_775 7_766 ?
O11 Na1 O1W 95.9(3) 2_755 7_766 ?
O11 Na1 O1W 166.8(3) . 7_766 ?
O11 Na1 O1W 95.9(3) 3_775 8_666 ?
O11 Na1 O1W 166.8(3) 2_755 8_666 ?
O11 Na1 O1W 82.1(3) . 8_666 ?
O1W Na1 O1W 97.3(3) 7_766 8_666 ?
O11 Na1 O1W 166.8(3) 3_775 9_656 ?
O11 Na1 O1W 82.1(3) 2_755 9_656 ?
O11 Na1 O1W 95.9(3) . 9_656 ?
O1W Na1 O1W 97.3(3) 7_766 9_656 ?
O1W Na1 O1W 97.3(3) 8_666 9_656 ?
O11 Na1 Na3 63.71(18) 3_775 7_766 ?
O11 Na1 Na3 148.0(3) 2_755 7_766 ?
O11 Na1 Na3 97.3(2) . 7_766 ?
O1W Na1 Na3 75.1(3) 7_766 7_766 ?
O1W Na1 Na3 37.2(3) 8_666 7_766 ?
O1W Na1 Na3 129.0(2) 9_656 7_766 ?
O11 Na1 Na3 97.3(2) 3_775 9_656 ?
O11 Na1 Na3 63.71(18) 2_755 9_656 ?
O11 Na1 Na3 148.0(3) . 9_656 ?
O1W Na1 Na3 37.2(3) 7_766 9_656 ?
O1W Na1 Na3 129.0(2) 8_666 9_656 ?
O1W Na1 Na3 75.1(3) 9_656 9_656 ?
Na3 Na1 Na3 112.35(7) 7_766 9_656 ?
O11 Na1 Na3 148.0(3) 3_775 8_666 ?
O11 Na1 Na3 97.3(2) 2_755 8_666 ?
O11 Na1 Na3 63.71(18) . 8_666 ?
O1W Na1 Na3 129.0(2) 7_766 8_666 ?
O1W Na1 Na3 75.1(3) 8_666 8_666 ?
O1W Na1 Na3 37.2(3) 9_656 8_666 ?
Na3 Na1 Na3 112.34(7) 7_766 8_666 ?
Na3 Na1 Na3 112.34(7) 9_656 8_666 ?
O15 Na2 O15 74.1(3) 5_656 6_556 ?
O15 Na2 O15 104.2(3) 5_656 . ?
O15 Na2 O15 177.2(4) 6_556 . ?
O15 Na2 O15 74.1(3) 5_656 4_666 ?
O15 Na2 O15 74.1(3) 6_556 4_666 ?
O15 Na2 O15 107.7(4) . 4_666 ?
O15 Na2 O15 107.7(4) 5_656 3_665 ?
O15 Na2 O15 104.2(3) 6_556 3_665 ?
O15 Na2 O15 74.1(3) . 3_665 ?
O15 Na2 O15 177.2(4) 4_666 3_665 ?
O15 Na2 O15 177.2(3) 5_656 2_655 ?
O15 Na2 O15 107.7(4) 6_556 2_655 ?
O15 Na2 O15 74.1(3) . 2_655 ?
O15 Na2 O15 104.2(3) 4_666 2_655 ?
O15 Na2 O15 74.1(3) 3_665 2_655 ?
O15 Na2 Ni2 44.09(18) 5_656 4_666 ?
O15 Na2 Ni2 44.09(18) 6_556 4_666 ?
O15 Na2 Ni2 135.91(18) . 4_666 ?
O15 Na2 Ni2 44.09(18) 4_666 4_666 ?
O15 Na2 Ni2 135.92(18) 3_665 4_666 ?
O15 Na2 Ni2 135.92(18) 2_655 4_666 ?
O15 Na2 Ni2 135.91(18) 5_656 . ?
O15 Na2 Ni2 135.91(18) 6_556 . ?
O15 Na2 Ni2 44.09(18) . . ?
O15 Na2 Ni2 135.91(18) 4_666 . ?
O15 Na2 Ni2 44.08(18) 3_665 . ?
O15 Na2 Ni2 44.08(18) 2_655 . ?
Ni2 Na2 Ni2 180.0 4_666 . ?
O1 Na3 O9 160.3(3) . 9_546 ?
O1 Na3 O2 102.5(3) . 7_656 ?
O9 Na3 O2 65.6(2) 9_546 7_656 ?
O1 Na3 O3 129.9(3) . 9_546 ?
O9 Na3 O3 64.8(2) 9_546 9_546 ?
O2 Na3 O3 76.9(2) 7_656 9_546 ?
O1 Na3 O1W 75.0(2) . 2_655 ?
O9 Na3 O1W 90.9(2) 9_546 2_655 ?
O2 Na3 O1W 99.0(3) 7_656 2_655 ?
O3 Na3 O1W 155.0(3) 9_546 2_655 ?
O1 Na3 O4 75.2(2) . 7_656 ?
O9 Na3 O4 109.1(2) 9_546 7_656 ?
O2 Na3 O4 60.7(2) 7_656 7_656 ?
O3 Na3 O4 60.9(2) 9_546 7_656 ?
O1W Na3 O4 138.6(3) 2_655 7_656 ?
O1 Na3 O5W 92.2(3) . 8_666 ?
O9 Na3 O5W 95.3(3) 9_546 8_666 ?
O2 Na3 O5W 157.5(3) 7_656 8_666 ?
O3 Na3 O5W 106.6(3) 9_546 8_666 ?
O1W Na3 O5W 68.2(3) 2_655 8_666 ?
O4 Na3 O5W 140.8(3) 7_656 8_666 ?
O1 Na3 W2 164.7(2) . 9_546 ?
O9 Na3 W2 32.91(13) 9_546 9_546 ?
O2 Na3 W2 77.88(17) 7_656 9_546 ?
O3 Na3 W2 34.84(14) 9_546 9_546 ?
O1W Na3 W2 120.24(19) 2_655 9_546 ?
O4 Na3 W2 92.13(17) 7_656 9_546 ?
O5W Na3 W2 92.4(3) 8_666 9_546 ?
O1 Na3 W3 130.4(3) . 9_546 ?
O9 Na3 W3 32.64(17) 9_546 9_546 ?
O2 Na3 W3 35.53(13) 7_656 9_546 ?
O3 Na3 W3 76.54(16) 9_546 9_546 ?
O1W Na3 W3 85.97(19) 2_655 9_546 ?
O4 Na3 W3 92.05(16) 7_656 9_546 ?
O5W Na3 W3 122.6(3) 8_666 9_546 ?
W2 Na3 W3 57.26(6) 9_546 9_546 ?
O1 Na3 W1 82.35(18) . 7_656 ?
O9 Na3 W1 91.4(2) 9_546 7_656 ?
O2 Na3 W1 29.71(13) 7_656 7_656 ?
O3 Na3 W1 73.77(19) 9_546 7_656 ?
O1W Na3 W1 114.6(2) 2_655 7_656 ?
O4 Na3 W1 32.92(15) 7_656 7_656 ?
O5W Na3 W1 172.7(3) 8_666 7_656 ?
W2 Na3 W1 91.66(8) 9_546 7_656 ?
W3 Na3 W1 64.64(7) 9_546 7_656 ?
O1 Na3 W1 100.87(18) . 9_546 ?
O9 Na3 W1 91.14(18) 9_546 9_546 ?
O2 Na3 W1 74.35(17) 7_656 9_546 ?
O3 Na3 W1 29.75(15) 9_546 9_546 ?
O1W Na3 W1 171.5(2) 2_655 9_546 ?
O4 Na3 W1 33.33(15) 7_656 9_546 ?
O5W Na3 W1 119.8(3) 8_666 9_546 ?
W2 Na3 W1 64.25(8) 9_546 9_546 ?
W3 Na3 W1 91.34(8) 9_546 9_546 ?
W1 Na3 W1 57.03(5) 7_656 9_546 ?
O1 Na3 Na6 117.8(3) . 7_756 ?
O9 Na3 Na6 76.6(3) 9_546 7_756 ?
O2 Na3 Na6 139.4(3) 7_656 7_756 ?
O3 Na3 Na6 73.8(2) 9_546 7_756 ?
O1W Na3 Na6 95.88(18) 2_655 7_756 ?
O4 Na3 Na6 123.4(2) 7_656 7_756 ?
O5W Na3 Na6 33.2(3) 8_666 7_756 ?
W2 Na3 Na6 62.0(2) 9_546 7_756 ?
W3 Na3 Na6 109.2(3) 9_546 7_756 ?
W1 Na3 Na6 147.53(16) 7_656 7_756 ?
W1 Na3 Na6 92.64(12) 9_546 7_756 ?
O7 Na4 O14 76.4(3) . . ?
O7 Na4 O3W 81.8(3) . . ?
O14 Na4 O3W 94.2(4) . . ?
O7 Na4 O2W 86.5(3) . . ?
O14 Na4 O2W 162.3(3) . . ?
O3W Na4 O2W 87.7(4) . . ?
O7 Na4 O6W 168.5(4) . . ?
O14 Na4 O6W 108.7(4) . . ?
O3W Na4 O6W 87.4(4) . . ?
O2W Na4 O6W 89.0(4) . . ?
O7 Na4 O6W 102.7(3) . 2_645 ?
O14 Na4 O6W 91.6(4) . 2_645 ?
O3W Na4 O6W 173.4(5) . 2_645 ?
O2W Na4 O6W 87.8(4) . 2_645 ?
O6W Na4 O6W 87.7(5) . 2_645 ?
O7 Na4 Ni1 37.8(2) . . ?
O14 Na4 Ni1 38.76(18) . . ?
O3W Na4 Ni1 84.9(3) . . ?
O2W Na4 Ni1 124.3(3) . . ?
O6W Na4 Ni1 145.4(4) . . ?
O6W Na4 Ni1 101.6(3) 2_645 . ?
O7 Na4 Na5 88.9(3) . . ?
O14 Na4 Na5 49.2(2) . . ?
O3W Na4 Na5 48.5(3) . . ?
O2W Na4 Na5 136.1(3) . . ?
O6W Na4 Na5 87.1(3) . . ?
O6W Na4 Na5 135.6(4) 2_645 . ?
Ni1 Na4 Na5 62.89(17) . . ?
O7 Na4 Na4 128.9(2) . 3_765 ?
O14 Na4 Na4 153.9(2) . 3_765 ?
O3W Na4 Na4 84.9(4) . 3_765 ?
O2W Na4 Na4 43.80(19) . 3_765 ?
O6W Na4 Na4 45.2(3) . 3_765 ?
O6W Na4 Na4 88.5(3) 2_645 3_765 ?
Ni1 Na4 Na4 164.64(10) . 3_765 ?
Na5 Na4 Na4 117.1(3) . 3_765 ?
O7 Na4 Na4 94.7(2) . 2_645 ?
O14 Na4 Na4 132.3(2) . 2_645 ?
O3W Na4 Na4 131.4(3) . 2_645 ?
O2W Na4 Na4 43.80(19) . 2_645 ?
O6W Na4 Na4 89.3(3) . 2_645 ?
O6W Na4 Na4 44.1(3) 2_645 2_645 ?
Ni1 Na4 Na4 120.53(19) . 2_645 ?
Na5 Na4 Na4 176.4(2) . 2_645 ?
Na4 Na4 Na4 60.001(3) 3_765 2_645 ?
O12 Na5 O4W 88.0(3) . . ?
O12 Na5 O3W 75.1(3) . . ?
O4W Na5 O3W 88.9(3) . . ?
O12 Na5 O14 71.5(2) . . ?
O4W Na5 O14 159.2(4) . . ?
O3W Na5 O14 89.0(3) . . ?
O12 Na5 Cl2 95.5(4) . . ?
O4W Na5 Cl2 91.7(3) . . ?
O3W Na5 Cl2 170.6(4) . . ?
O14 Na5 Cl2 87.0(3) . . ?
O12 Na5 Cl2 156.9(4) . 2_755 ?
O4W Na5 Cl2 90.5(3) . 2_755 ?
O3W Na5 Cl2 81.8(4) . 2_755 ?
O14 Na5 Cl2 109.7(4) . 2_755 ?
Cl2 Na5 Cl2 107.6(4) . 2_755 ?
O12 Na5 Na4 79.8(2) . . ?
O4W Na5 Na4 135.6(3) . . ?
O3W Na5 Na4 46.7(2) . . ?
O14 Na5 Na4 45.6(2) . . ?
Cl2 Na5 Na4 131.6(3) . . ?
Cl2 Na5 Na4 85.3(3) 2_755 . ?
O12 Na5 Ni1 35.04(15) . . ?
O4W Na5 Ni1 122.9(3) . . ?
O3W Na5 Ni1 80.4(2) . . ?
O14 Na5 Ni1 36.46(17) . . ?
Cl2 Na5 Ni1 91.3(3) . . ?
Cl2 Na5 Ni1 141.5(3) 2_755 . ?
Na4 Na5 Ni1 57.97(14) . . ?
O12 Na5 Na5 97.3(4) . 3_775 ?
O4W Na5 Na5 43.62(18) . 3_775 ?
O3W Na5 Na5 132.5(3) . 3_775 ?
O14 Na5 Na5 133.7(5) . 3_775 ?
Cl2 Na5 Na5 48.5(3) . 3_775 ?
Cl2 Na5 Na5 97.4(3) 2_755 3_775 ?
Na4 Na5 Na5 177.2(3) . 3_775 ?
Ni1 Na5 Na5 119.7(4) . 3_775 ?
O12 Na5 Na5 129.62(19) . 2_755 ?
O4W Na5 Na5 43.62(18) . 2_755 ?
O3W Na5 Na5 88.6(3) . 2_755 ?
O14 Na5 Na5 157.0(4) . 2_755 ?
Cl2 Na5 Na5 98.3(3) . 2_755 ?
Cl2 Na5 Na5 47.3(3) 2_755 2_755 ?
Na4 Na5 Na5 121.7(4) . 2_755 ?
Ni1 Na5 Na5 163.25(11) . 2_755 ?
Na5 Na5 Na5 60.000(3) 3_775 2_755 ?
O5W Na6 O5W 95.7(7) 3_765 . ?
O5W Na6 O5W 95.7(7) 3_765 2_645 ?
O5W Na6 O5W 95.7(7) . 2_645 ?
O5W Na6 O6 78.9(4) 3_765 3_765 ?
O5W Na6 O6 157.0(5) . 3_765 ?
O5W Na6 O6 107.0(4) 2_645 3_765 ?
O5W Na6 O6 157.0(5) 3_765 2_645 ?
O5W Na6 O6 107.0(4) . 2_645 ?
O5W Na6 O6 78.9(4) 2_645 2_645 ?
O6 Na6 O6 81.4(6) 3_765 2_645 ?
O5W Na6 O6 107.0(4) 3_765 . ?
O5W Na6 O6 78.9(4) . . ?
O5W Na6 O6 157.0(5) 2_645 . ?
O6 Na6 O6 81.4(6) 3_765 . ?
O6 Na6 O6 81.4(6) 2_645 . ?
O5W Na6 O7W 58.9(5) 3_765 . ?
O5W Na6 O7W 58.9(5) . . ?
O5W Na6 O7W 58.9(5) 2_645 . ?
O6 Na6 O7W 131.1(4) 3_765 . ?
O6 Na6 O7W 131.1(4) 2_645 . ?
O6 Na6 O7W 131.1(4) . . ?
O5W Na6 Na3 71.4(4) 3_765 7_756 ?
O5W Na6 Na3 132.1(7) . 7_756 ?
O5W Na6 Na3 43.3(4) 2_645 7_756 ?
O6 Na6 Na3 67.63(18) 3_765 7_756 ?
O6 Na6 Na3 90.31(16) 2_645 7_756 ?
O6 Na6 Na3 148.8(6) . 7_756 ?
O7W Na6 Na3 75.9(3) . 7_756 ?
O5W Na6 Na3 43.3(4) 3_765 8_666 ?
O5W Na6 Na3 71.4(4) . 8_666 ?
O5W Na6 Na3 132.1(7) 2_645 8_666 ?
O6 Na6 Na3 90.31(16) 3_765 8_666 ?
O6 Na6 Na3 148.8(6) 2_645 8_666 ?
O6 Na6 Na3 67.63(18) . 8_666 ?
O7W Na6 Na3 75.9(3) . 8_666 ?
Na3 Na6 Na3 114.3(2) 7_756 8_666 ?
O5W Na6 Na3 132.1(7) 3_765 9_546 ?
O5W Na6 Na3 43.3(4) . 9_546 ?
O5W Na6 Na3 71.4(4) 2_645 9_546 ?
O6 Na6 Na3 148.8(6) 3_765 9_546 ?
O6 Na6 Na3 67.63(18) 2_645 9_546 ?
O6 Na6 Na3 90.31(17) . 9_546 ?
O7W Na6 Na3 75.9(3) . 9_546 ?
Na3 Na6 Na3 114.3(2) 7_756 9_546 ?
Na3 Na6 Na3 114.3(2) 8_666 9_546 ?
Na5 Cl2 Na5 84.2(3) . 3_775 ?
Na1 O1W Na3 112.1(3) 7_766 3_665 ?
Na4 O2W Na4 92.4(4) 3_765 2_645 ?
Na4 O2W Na4 92.4(4) 3_765 . ?
Na4 O2W Na4 92.4(4) 2_645 . ?
Na4 O3W Na5 84.8(4) . . ?
Na5 O4W Na5 92.8(4) 3_775 2_755 ?
Na5 O4W Na5 92.7(4) 3_775 . ?
Na5 O4W Na5 92.8(4) 2_755 . ?
Na6 O5W Na3 103.5(6) . 9_546 ?
Na4 O6W Na4 90.7(4) . 3_765 ?
Na6 O7W Na6 179.999(1) . 7_756 ?
O9W O8W O9W 74(6) 4_666 6_566 ?
O9W O8W O9W 74(6) 4_666 5_556 ?
O9W O8W O9W 74(6) 6_566 5_556 ?
O9W O8W O9W 130(8) 4_666 . ?
O9W O8W O9W 93(7) 6_566 . ?
O9W O8W O9W 149(8) 5_556 . ?
O9W O8W O9W 93(8) 4_666 3_565 ?
O9W O8W O9W 149(7) 6_566 3_565 ?
O9W O8W O9W 130(9) 5_556 3_565 ?
O9W O8W O9W 74(6) . 3_565 ?
O9W O8W O9W 149(8) 4_666 2_665 ?
O9W O8W O9W 130(9) 6_566 2_665 ?
O9W O8W O9W 93(7) 5_556 2_665 ?
O9W O8W O9W 74(6) . 2_665 ?
O9W O8W O9W 74(6) 3_565 2_665 ?
O8W O9W O9W 53(3) . 3_565 ?
O8W O9W O9W 53(3) . 2_665 ?
O9W O9W O9W 60.00(11) 3_565 2_665 ?
O8W O9W O9W 44(4) . 6_566 ?
O9W O9W O9W 92.7(16) 3_565 6_566 ?
O9W O9W O9W 86(4) 2_665 6_566 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1 1.725(7) . ?
W1 O2 1.853(5) . ?
W1 O3 1.866(6) . ?
W1 O4 1.939(7) . ?
W1 O4 1.971(7) 2_655 ?
W1 O5 2.340(6) . ?
W1 Na3 3.543(4) 7_656 ?
W1 Na3 3.562(4) 8_666 ?
W2 O6 1.733(8) . ?
W2 O7 1.796(6) . ?
W2 O8 1.909(6) . ?
W2 O9 1.949(5) . ?
W2 O3 2.019(6) . ?
W2 O10 2.355(7) . ?
W2 Na3 3.477(4) 8_666 ?
W3 O11 1.727(6) . ?
W3 O12 1.790(6) . ?
W3 O8 1.897(6) 2_655 ?
W3 O9 1.954(7) . ?
W3 O2 2.066(5) 2_655 ?
W3 O10 2.298(5) . ?
W3 Na3 3.500(4) 8_666 ?
Ni1 O13 2.002(7) . ?
Ni1 O13 2.038(7) 3_665 ?
Ni1 O12 2.048(5) . ?
Ni1 O7 2.054(7) . ?
Ni1 O14 2.076(7) . ?
Ni1 O10 2.212(6) . ?
Ni1 Ni2 2.9038(17) . ?
Ni1 Na4 3.304(7) . ?
Ni1 Na5 3.469(6) . ?
Ni2 O15 2.041(7) 3_665 ?
Ni2 O15 2.041(8) 2_655 ?
Ni2 O15 2.041(7) . ?
Ni2 O13 2.048(5) . ?
Ni2 O13 2.049(5) 3_665 ?
Ni2 O13 2.049(5) 2_655 ?
Ni2 Ni1 2.9038(17) 2_655 ?
Ni2 Ni1 2.9038(17) 3_665 ?
Ni2 Na2 2.9160(18) . ?
Si1 O10 1.639(6) 2_655 ?
Si1 O10 1.639(7) 3_665 ?
Si1 O10 1.639(6) . ?
Si1 O5 1.667(11) . ?
O1 Na3 2.361(7) . ?
O2 W3 2.066(5) 3_665 ?
O2 Na3 2.486(7) 7_656 ?
O3 Na3 2.496(7) 8_666 ?
O4 W1 1.971(7) 3_665 ?
O4 Na3 2.745(6) 7_656 ?
O5 W1 2.340(6) 2_655 ?
O5 W1 2.340(6) 3_665 ?
O6 Na6 2.291(15) . ?
O7 Na4 2.267(9) . ?
O8 W3 1.897(6) 3_665 ?
O9 Na3 2.442(7) 8_666 ?
O11 Na1 2.180(7) . ?
O12 Na5 2.365(9) . ?
O13 Ni1 2.038(7) 2_655 ?
O14 C1 1.274(12) 3_665 ?
O14 Na4 2.398(10) . ?
O14 Na5 2.543(8) . ?
O15 C1 1.273(15) . ?
O15 Na2 2.321(7) . ?
C1 O14 1.274(12) 2_655 ?
C1 C2 1.516(16) . ?
C2 H2A 0.9600 . ?
C2 H2B 0.9600 . ?
C2 H2C 0.9600 . ?
Na1 O11 2.180(7) 3_775 ?
Na1 O11 2.180(7) 2_755 ?
Na1 O1W 2.297(9) 7_766 ?
Na1 O1W 2.297(9) 8_666 ?
Na1 O1W 2.297(9) 9_656 ?
Na1 Na3 4.174(5) 7_766 ?
Na1 Na3 4.174(5) 9_656 ?
Na1 Na3 4.174(6) 8_666 ?
Na2 O15 2.321(7) 5_656 ?
Na2 O15 2.321(7) 6_556 ?
Na2 O15 2.321(7) 4_666 ?
Na2 O15 2.321(7) 3_665 ?
Na2 O15 2.321(7) 2_655 ?
Na2 Ni2 2.9159(18) 4_666 ?
Na3 O9 2.442(7) 9_546 ?
Na3 O2 2.486(8) 7_656 ?
Na3 O3 2.496(7) 9_546 ?
Na3 O1W 2.726(13) 2_655 ?
Na3 O4 2.745(6) 7_656 ?
Na3 O5W 2.786(13) 8_666 ?
Na3 W2 3.477(4) 9_546 ?
Na3 W3 3.500(4) 9_546 ?
Na3 W1 3.543(4) 7_656 ?
Na3 W1 3.562(4) 9_546 ?
Na3 Na6 3.952(7) 7_756 ?
Na4 O3W 2.446(9) . ?
Na4 O2W 2.479(9) . ?
Na4 O6W 2.490(14) . ?
Na4 O6W 2.541(14) 2_645 ?
Na4 Na5 3.346(9) . ?
Na4 Na4 3.579(11) 3_765 ?
Na4 Na4 3.579(11) 2_645 ?
Na5 O4W 2.453(8) . ?
Na5 O3W 2.515(14) . ?
Na5 Cl2 2.623(12) . ?
Na5 Cl2 2.674(10) 2_755 ?
Na5 Na5 3.551(10) 3_775 ?
Na5 Na5 3.551(10) 2_755 ?
Na6 O5W 2.225(14) 3_765 ?
Na6 O5W 2.225(14) . ?
Na6 O5W 2.225(14) 2_645 ?
Na6 O6 2.291(15) 3_765 ?
Na6 O6 2.291(15) 2_645 ?
Na6 O7W 2.754(19) . ?
Na6 Na3 3.952(7) 7_756 ?
Na6 Na3 3.952(7) 8_666 ?
Na6 Na3 3.952(7) 9_546 ?
Cl2 Na5 2.674(10) 3_775 ?
O1W Na1 2.297(9) 7_766 ?
O1W Na3 2.726(13) 3_665 ?
O2W Na4 2.479(9) 3_765 ?
O2W Na4 2.479(9) 2_645 ?
O4W Na5 2.453(8) 3_775 ?
O4W Na5 2.453(8) 2_755 ?
O5W Na3 2.786(13) 9_546 ?
O6W Na4 2.541(14) 3_765 ?
O7W Na6 2.754(19) 7_756 ?
O8W O9W 1.07(7) 4_666 ?
O8W O9W 1.07(7) 6_566 ?
O8W O9W 1.07(7) 5_556 ?
O8W O9W 1.07(7) . ?
O8W O9W 1.07(7) 3_565 ?
O8W O9W 1.07(7) 2_665 ?
O9W O9W 1.29(9) 3_565 ?
O9W O9W 1.29(9) 2_665 ?
O9W O9W 1.56(18) 6_566 ?
